#------------------------------------------------------------------------------
#$Date: 2023-03-31 16:04:01 +0300 (Fri, 31 Mar 2023) $
#$Revision: 282155 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/02/27/2022708.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2022708
loop_
_publ_author_name
'Pavlyuk, Nazar'
'Dmytriv, Grygoriy'
'Pavlyuk, Volodymyr'
'Chumak, Ihor'
'Indris, Sylvio'
'Schwarz, Bjoern'
'Ehrenberg, Helmut'
_publ_section_title
;
 MgMn₄Ga₁₈: a novel three-shell gallium cluster structure
;
_journal_coeditor_code           YP3224
_journal_issue                   8
_journal_name_full               'Acta Crystallographica, Section C'
_journal_page_first              455
_journal_page_last               461
_journal_paper_doi               10.1107/S2053229622007185
_journal_volume                  78
_journal_year                    2022
_chemical_formula_iupac          'Mg Mn4 Ga18'
_chemical_formula_moiety         '2(Ga9 Mn2), Mg'
_chemical_formula_sum            'Ga18 Mg Mn4'
_chemical_formula_weight         1499.03
_space_group_crystal_system      tetragonal
_space_group_IT_number           123
_space_group_name_Hall           '-P 4 2'
_space_group_name_H-M_alt        'P 4/m m m'
_atom_sites_solution_hydrogens   .
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   6.3116(9)
_cell_length_b                   6.3116(9)
_cell_length_c                   9.944(2)
_cell_measurement_reflns_used    250
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      26.333
_cell_measurement_theta_min      2.048
_cell_volume                     396.13(11)
_computing_cell_refinement
;
CrysAlis PRO (Rigaku OD, 2015)
;
_computing_data_collection
;
CrysAlis PRO (Rigaku OD, 2015)
;
_computing_data_reduction
;
CrysAlis PRO (Rigaku OD, 2015)
;
_computing_molecular_graphics
;
DIAMOND (Brandenburg, 2006)
;
_computing_publication_material
;
SHELX97 (Sheldrick, 2008)
;
_computing_structure_refinement
;
SHELXL2014 (Sheldrick, 2015b)
;
_computing_structure_solution
;
SHELXT2014 (Sheldrick, 2015a)
;
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0656
_diffrn_reflns_av_unetI/netI     0.0237
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            5352
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.333
_diffrn_reflns_theta_min         2.048
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    33.081
_exptl_absorpt_correction_T_max  0.513
_exptl_absorpt_correction_T_min  0.221
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
(CrysAlis RED; Oxford Diffraction, 2008)
;
_exptl_crystal_colour            'metallic dark grey'
_exptl_crystal_density_diffrn    6.284
_exptl_crystal_description       prism
_exptl_crystal_F_000             670
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.559
_refine_diff_density_min         -1.866
_refine_ls_extinction_coef       0.0036(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method
;
SHELXL2014 (Sheldrick, 2015b)
;
_refine_ls_goodness_of_fit_ref   1.410
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     27
_refine_ls_number_reflns         288
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.410
_refine_ls_R_factor_all          0.0522
_refine_ls_R_factor_gt           0.0444
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+14.5817P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0805
_refine_ls_wR_factor_ref         0.0823
_reflns_number_gt                250
_reflns_number_total             288
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            yp3224sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        396.13(14)
_cod_database_code               2022708
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ga Ga1 0.23869(17) 0.23869(17) 0.23605(15) 0.0173(5) Uani d 1 . .
Ga Ga2 0.5000 0.5000 0.3872(4) 0.0558(17) Uani d 1 . .
Ga Ga3 0.3110(4) 0.0000 0.5000 0.0231(7) Uani d 1 . .
Ga Ga4 0.1870(4) 0.5000 0.0000 0.0183(6) Uani d 1 . .
Mn Mn1 0.0000 0.0000 0.3433(4) 0.0059(9) Uani d 1 . .
Mn Mn2 0.5000 0.5000 0.1526(4) 0.0077(9) Uani d 1 . .
Mg Mg1 0.0000 0.0000 0.0000 0.033(4) Uani d 1 . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Mn1 Ga1 Mn2 . . 173.00(15)
Mn1 Ga1 Ga2 . . 120.62(13)
Mn2 Ga1 Ga2 . . 52.38(11)
Mn1 Ga1 Ga4 . . 130.82(10)
Mn2 Ga1 Ga4 . . 54.70(8)
Ga2 Ga1 Ga4 . . 99.66(8)
Mn1 Ga1 Ga4 . 3_655 130.82(10)
Mn2 Ga1 Ga4 . 3_655 54.70(8)
Ga2 Ga1 Ga4 . 3_655 99.66(8)
Ga4 Ga1 Ga4 . 3_655 57.86(8)
Mn1 Ga1 Ga1 . 4 50.78(4)
Mn2 Ga1 Ga1 . 4 131.77(3)
Ga2 Ga1 Ga1 . 4 126.47(4)
Ga4 Ga1 Ga1 . 4 124.84(3)
Ga4 Ga1 Ga1 3_655 4 83.52(5)
Mn1 Ga1 Ga1 . 3 50.78(4)
Mn2 Ga1 Ga1 . 3 131.77(3)
Ga2 Ga1 Ga1 . 3 126.47(4)
Ga4 Ga1 Ga1 . 3 83.52(5)
Ga4 Ga1 Ga1 3_655 3 124.84(3)
Ga1 Ga1 Ga1 4 3 90.0
Mn1 Ga1 Mg1 . . 74.36(10)
Mn2 Ga1 Mg1 . . 112.64(10)
Ga2 Ga1 Mg1 . . 165.02(9)
Ga4 Ga1 Mg1 . . 67.41(4)
Ga4 Ga1 Mg1 3_655 . 67.41(4)
Ga1 Ga1 Mg1 4 . 61.625(16)
Ga1 Ga1 Mg1 3 . 61.625(16)
Ga2 Ga2 Mn2 9_666 . 180.0
Ga2 Ga2 Ga1 9_666 . 122.79(8)
Mn2 Ga2 Ga1 . . 57.21(8)
Ga2 Ga2 Ga1 9_666 2_665 122.79(8)
Mn2 Ga2 Ga1 . 2_665 57.21(8)
Ga1 Ga2 Ga1 . 2_665 114.42(15)
Ga2 Ga2 Ga1 9_666 3_655 122.79(8)
Mn2 Ga2 Ga1 . 3_655 57.21(8)
Ga1 Ga2 Ga1 . 3_655 72.94(7)
Ga1 Ga2 Ga1 2_665 3_655 72.95(7)
Ga2 Ga2 Ga1 9_666 4_565 122.79(8)
Mn2 Ga2 Ga1 . 4_565 57.21(8)
Ga1 Ga2 Ga1 . 4_565 72.94(7)
Ga1 Ga2 Ga1 2_665 4_565 72.95(7)
Ga1 Ga2 Ga1 3_655 4_565 114.42(15)
Ga3 Ga3 Mn1 9_656 . 141.55(8)
Ga3 Ga3 Mn1 9_656 9_556 141.55(8)
Mn1 Ga3 Mn1 . 9_556 76.89(16)
Ga3 Ga3 Ga3 9_656 11_556 135.0
Mn1 Ga3 Ga3 . 11_556 56.37(4)
Mn1 Ga3 Ga3 9_556 11_556 56.37(4)
Ga3 Ga3 Ga3 9_656 3 135.0
Mn1 Ga3 Ga3 . 3 56.37(4)
Mn1 Ga3 Ga3 9_556 3 56.37(4)
Ga3 Ga3 Ga3 11_556 3 90.0000(10)
Ga4 Ga4 Mn2 9_565 9_665 142.47(8)
Ga4 Ga4 Mn2 9_565 . 142.47(8)
Mn2 Ga4 Mn2 9_665 . 75.06(16)
Ga4 Ga4 Ga4 9_565 11_565 135.0
Mn2 Ga4 Ga4 9_665 11_565 55.89(4)
Mn2 Ga4 Ga4 . 11_565 55.89(4)
Ga4 Ga4 Ga4 9_565 3_655 135.0
Mn2 Ga4 Ga4 9_665 3_655 55.89(4)
Mn2 Ga4 Ga4 . 3_655 55.89(4)
Ga4 Ga4 Ga4 11_565 3_655 90.0
Ga4 Ga4 Ga1 9_565 . 96.48(5)
Mn2 Ga4 Ga1 9_665 . 113.94(9)
Mn2 Ga4 Ga1 . . 54.21(6)
Ga4 Ga4 Ga1 11_565 . 108.91(5)
Ga4 Ga4 Ga1 3_655 . 61.07(4)
Ga4 Ga4 Ga1 9_565 4_565 96.48(5)
Mn2 Ga4 Ga1 9_665 4_565 113.94(9)
Mn2 Ga4 Ga1 . 4_565 54.21(6)
Ga4 Ga4 Ga1 11_565 4_565 61.07(4)
Ga4 Ga4 Ga1 3_655 4_565 108.91(5)
Ga1 Ga4 Ga1 . 4_565 69.67(6)
Ga4 Ga4 Ga1 9_565 10 96.48(5)
Mn2 Ga4 Ga1 9_665 10 54.21(6)
Mn2 Ga4 Ga1 . 10 113.94(9)
Ga4 Ga4 Ga1 11_565 10 108.91(5)
Ga4 Ga4 Ga1 3_655 10 61.07(4)
Ga1 Ga4 Ga1 . 10 108.78(5)
Ga1 Ga4 Ga1 4_565 10 167.04(10)
Ga4 Ga4 Ga1 9_565 11_565 96.48(5)
Mn2 Ga4 Ga1 9_665 11_565 54.21(6)
Mn2 Ga4 Ga1 . 11_565 113.94(9)
Ga4 Ga4 Ga1 11_565 11_565 61.07(4)
Ga4 Ga4 Ga1 3_655 11_565 108.91(5)
Ga1 Ga4 Ga1 . 11_565 167.04(10)
Ga1 Ga4 Ga1 4_565 11_565 108.78(5)
Ga1 Ga4 Ga1 10 11_565 69.67(6)
Ga1 Mn1 Ga1 2 4 78.45(8)
Ga1 Mn1 Ga1 2 3 78.45(8)
Ga1 Mn1 Ga1 4 3 126.83(19)
Ga1 Mn1 Ga1 2 . 126.83(19)
Ga1 Mn1 Ga1 4 . 78.45(8)
Ga1 Mn1 Ga1 3 . 78.45(8)
Ga1 Mn1 Ga3 2 . 140.67(5)
Ga1 Mn1 Ga3 4 . 77.47(4)
Ga1 Mn1 Ga3 3 . 140.67(5)
Ga1 Mn1 Ga3 . . 77.47(4)
Ga1 Mn1 Ga3 2 3 140.67(5)
Ga1 Mn1 Ga3 4 3 140.67(5)
Ga1 Mn1 Ga3 3 3 77.47(4)
Ga1 Mn1 Ga3 . 3 77.47(4)
Ga3 Mn1 Ga3 . 3 67.26(9)
Ga1 Mn1 Ga3 2 11_556 77.47(4)
Ga1 Mn1 Ga3 4 11_556 77.47(4)
Ga1 Mn1 Ga3 3 11_556 140.67(5)
Ga1 Mn1 Ga3 . 11_556 140.67(5)
Ga3 Mn1 Ga3 . 11_556 67.26(9)
Ga3 Mn1 Ga3 3 11_556 103.11(16)
Ga1 Mn1 Ga3 2 9_556 77.47(4)
Ga1 Mn1 Ga3 4 9_556 140.67(5)
Ga1 Mn1 Ga3 3 9_556 77.47(4)
Ga1 Mn1 Ga3 . 9_556 140.67(5)
Ga3 Mn1 Ga3 . 9_556 103.11(16)
Ga3 Mn1 Ga3 3 9_556 67.26(9)
Ga3 Mn1 Ga3 11_556 9_556 67.26(9)
Ga1 Mn1 Mn1 2 9_556 116.59(9)
Ga1 Mn1 Mn1 4 9_556 116.59(9)
Ga1 Mn1 Mn1 3 9_556 116.59(9)
Ga1 Mn1 Mn1 . 9_556 116.59(9)
Ga3 Mn1 Mn1 . 9_556 51.55(8)
Ga3 Mn1 Mn1 3 9_556 51.55(8)
Ga3 Mn1 Mn1 11_556 9_556 51.55(8)
Ga3 Mn1 Mn1 9_556 9_556 51.55(8)
Ga1 Mn1 Mg1 2 . 63.41(9)
Ga1 Mn1 Mg1 4 . 63.41(9)
Ga1 Mn1 Mg1 3 . 63.41(9)
Ga1 Mn1 Mg1 . . 63.41(9)
Ga3 Mn1 Mg1 . . 128.45(8)
Ga3 Mn1 Mg1 3 . 128.45(8)
Ga3 Mn1 Mg1 11_556 . 128.45(8)
Ga3 Mn1 Mg1 9_556 . 128.45(8)
Mn1 Mn1 Mg1 9_556 . 180.0
Ga2 Mn2 Ga1 . . 70.41(9)
Ga2 Mn2 Ga1 . 2_665 70.41(9)
Ga1 Mn2 Ga1 . 2_665 140.82(18)
Ga2 Mn2 Ga1 . 4_565 70.41(9)
Ga1 Mn2 Ga1 . 4_565 83.55(6)
Ga1 Mn2 Ga1 2_665 4_565 83.55(6)
Ga2 Mn2 Ga1 . 3_655 70.41(9)
Ga1 Mn2 Ga1 . 3_655 83.55(6)
Ga1 Mn2 Ga1 2_665 3_655 83.55(6)
Ga1 Mn2 Ga1 4_565 3_655 140.82(18)
Ga2 Mn2 Ga4 . . 127.53(8)
Ga1 Mn2 Ga4 . . 71.09(4)
Ga1 Mn2 Ga4 2_665 . 137.10(7)
Ga1 Mn2 Ga4 4_565 . 71.09(4)
Ga1 Mn2 Ga4 3_655 . 137.10(7)
Ga2 Mn2 Ga4 . 3_655 127.53(8)
Ga1 Mn2 Ga4 . 3_655 71.09(4)
Ga1 Mn2 Ga4 2_665 3_655 137.10(7)
Ga1 Mn2 Ga4 4_565 3_655 137.10(7)
Ga1 Mn2 Ga4 3_655 3_655 71.09(4)
Ga4 Mn2 Ga4 . 3_655 68.22(8)
Ga2 Mn2 Ga4 . 11_565 127.53(8)
Ga1 Mn2 Ga4 . 11_565 137.10(7)
Ga1 Mn2 Ga4 2_665 11_565 71.09(4)
Ga1 Mn2 Ga4 4_565 11_565 71.09(4)
Ga1 Mn2 Ga4 3_655 11_565 137.10(7)
Ga4 Mn2 Ga4 . 11_565 68.22(8)
Ga4 Mn2 Ga4 3_655 11_565 104.94(16)
Ga2 Mn2 Ga4 . 9_665 127.53(8)
Ga1 Mn2 Ga4 . 9_665 137.10(7)
Ga1 Mn2 Ga4 2_665 9_665 71.09(4)
Ga1 Mn2 Ga4 4_565 9_665 137.10(7)
Ga1 Mn2 Ga4 3_655 9_665 71.09(4)
Ga4 Mn2 Ga4 . 9_665 104.94(16)
Ga4 Mn2 Ga4 3_655 9_665 68.22(8)
Ga4 Mn2 Ga4 11_565 9_665 68.22(8)
Ga2 Mn2 Mn2 . 9_665 180.0
Ga1 Mn2 Mn2 . 9_665 109.59(9)
Ga1 Mn2 Mn2 2_665 9_665 109.59(9)
Ga1 Mn2 Mn2 4_565 9_665 109.59(9)
Ga1 Mn2 Mn2 3_655 9_665 109.59(9)
Ga4 Mn2 Mn2 . 9_665 52.47(8)
Ga4 Mn2 Mn2 3_655 9_665 52.47(8)
Ga4 Mn2 Mn2 11_565 9_665 52.47(8)
Ga4 Mn2 Mn2 9_665 9_665 52.47(8)
Ga1 Mg1 Ga1 . 9 180.0
Ga1 Mg1 Ga1 . 12 123.25(3)
Ga1 Mg1 Ga1 9 12 56.75(3)
Ga1 Mg1 Ga1 . 4 56.75(3)
Ga1 Mg1 Ga1 9 4 123.25(3)
Ga1 Mg1 Ga1 12 4 180.0
Ga1 Mg1 Ga1 . 11 123.25(3)
Ga1 Mg1 Ga1 9 11 56.75(3)
Ga1 Mg1 Ga1 12 11 84.46(5)
Ga1 Mg1 Ga1 4 11 95.54(5)
Ga1 Mg1 Ga1 . 3 56.75(3)
Ga1 Mg1 Ga1 9 3 123.25(3)
Ga1 Mg1 Ga1 12 3 95.54(5)
Ga1 Mg1 Ga1 4 3 84.46(5)
Ga1 Mg1 Ga1 11 3 180.0
Ga1 Mg1 Ga1 . 2 84.46(5)
Ga1 Mg1 Ga1 9 2 95.54(5)
Ga1 Mg1 Ga1 12 2 123.25(3)
Ga1 Mg1 Ga1 4 2 56.75(3)
Ga1 Mg1 Ga1 11 2 123.25(3)
Ga1 Mg1 Ga1 3 2 56.75(3)
Ga1 Mg1 Ga1 . 10 95.54(5)
Ga1 Mg1 Ga1 9 10 84.46(5)
Ga1 Mg1 Ga1 12 10 56.75(3)
Ga1 Mg1 Ga1 4 10 123.25(3)
Ga1 Mg1 Ga1 11 10 56.75(3)
Ga1 Mg1 Ga1 3 10 123.25(3)
Ga1 Mg1 Ga1 2 10 180.0
Ga1 Mg1 Mn1 . 9 137.77(3)
Ga1 Mg1 Mn1 9 9 42.23(3)
Ga1 Mg1 Mn1 12 9 42.23(3)
Ga1 Mg1 Mn1 4 9 137.77(3)
Ga1 Mg1 Mn1 11 9 42.23(3)
Ga1 Mg1 Mn1 3 9 137.77(3)
Ga1 Mg1 Mn1 2 9 137.77(3)
Ga1 Mg1 Mn1 10 9 42.23(3)
Ga1 Mg1 Mn1 . . 42.23(3)
Ga1 Mg1 Mn1 9 . 137.77(3)
Ga1 Mg1 Mn1 12 . 137.77(3)
Ga1 Mg1 Mn1 4 . 42.23(3)
Ga1 Mg1 Mn1 11 . 137.77(3)
Ga1 Mg1 Mn1 3 . 42.23(3)
Ga1 Mg1 Mn1 2 . 42.23(3)
Ga1 Mg1 Mn1 10 . 137.77(3)
Mn1 Mg1 Mn1 9 . 180.0
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Ga1 Mn1 . 2.382(2)
Ga1 Mn2 . 2.4757(19)
Ga1 Ga2 . 2.775(3)
Ga1 Ga4 . 2.8873(14)
Ga1 Ga4 3_655 2.8873(14)
Ga1 Ga1 4 3.013(2)
Ga1 Ga1 3 3.013(2)
Ga1 Mg1 . 3.1700(16)
Ga2 Ga2 9_666 2.244(8)
Ga2 Mn2 . 2.333(6)
Ga2 Ga1 2_665 2.775(3)
Ga2 Ga1 3_655 2.775(3)
Ga2 Ga1 4_565 2.775(3)
Ga3 Ga3 9_656 2.386(5)
Ga3 Mn1 . 2.506(3)
Ga3 Mn1 9_556 2.506(3)
Ga3 Ga3 11_556 2.776(3)
Ga3 Ga3 3 2.776(3)
Ga4 Ga4 9_565 2.361(5)
Ga4 Mn2 9_665 2.491(3)
Ga4 Mn2 . 2.491(3)
Ga4 Ga4 11_565 2.793(3)
Ga4 Ga4 3_655 2.793(3)
Ga4 Ga1 4_565 2.8873(14)
Ga4 Ga1 10 2.8873(14)
Ga4 Ga1 11_565 2.8873(14)
Mn1 Ga1 2 2.382(2)
Mn1 Ga1 4 2.382(2)
Mn1 Ga1 3 2.382(2)
Mn1 Ga3 3 2.506(3)
Mn1 Ga3 11_556 2.506(3)
Mn1 Ga3 9_556 2.506(3)
Mn1 Mn1 9_556 3.117(8)
Mn1 Mg1 . 3.414(4)
Mn2 Ga1 2_665 2.4758(19)
Mn2 Ga1 4_565 2.4758(19)
Mn2 Ga1 3_655 2.4758(19)
Mn2 Ga4 3_655 2.491(3)
Mn2 Ga4 11_565 2.491(3)
Mn2 Ga4 9_665 2.491(3)
Mn2 Mn2 9_665 3.034(8)
Mg1 Ga1 9 3.1700(16)
Mg1 Ga1 12 3.1700(16)
Mg1 Ga1 4 3.1700(16)
Mg1 Ga1 11 3.1700(16)
Mg1 Ga1 3 3.1700(16)
Mg1 Ga1 2 3.1700(16)
Mg1 Ga1 10 3.1700(16)
Mg1 Mn1 9 3.414(4)

_cod_database_fobs_code 2022708
